APPLIED PHYSICS LETTERS 97, 042114 共2010兲
Mobility improvement in nanowire junctionless transistors by uniaxial strain Jean-Pierre Raskin,1,a兲 Jean-Pierre Colinge,2,b兲 Isabelle Ferain,2 Abhinav Kranti,2 Chi-Woo Lee,2 Nima Dehdashti Akhavan,2 Ran Yan,2 Pedram Razavi,2 and Ran Yu2 1
Information and Communication Technologies, Electronics and Applied Mathematics, Université catholique de Louvain, Place du Levant, 3, Maxwell Building, B-1348 Louvain-la-Neuve, Belgium 2 Tyndall National Institute, University College Cork, Dyke Parade, Cork, Ireland
共Received 15 May 2010; accepted 9 July 2010; published online 30 July 2010兲 Improvement of current drive in nand p-type silicon junctionless metal-oxide-semiconductor-ﬁeld-effect-transistors 共MOSFETs兲 using strain is demonstrated. Junctionless transistors have heavily doped channels with doping concentrations in excess of 1019 cm−3 and feature bulk conduction, as opposed to surface channel conduction. The extracted piezoresistance coefﬁcients are in good agreement with the piezoresistive theory and the published coefﬁcients for bulk silicon even for 10 nm thick silicon nanowires as narrow as 20 nm. These experimental results demonstrate the possibility of enhancing mobility in heavily doped silicon junctionless MOSFETs using strain technology. © 2010 American Institute of Physics. 关doi:10.1063/1.3474608兴 Mechanical strain is a widely used technique to increase carrier mobility in the channel of silicon metal-oxidesemiconductor-ﬁeld-effect-transistors 共MOSFETs兲. The technique has been applied to bulk MOSFETs,1 silicon-oninsulator 共SOI兲 transistors,2–4 as well as to multigate FETs 共MuGFETs兲.5 These studies demonstrate the great interest of strain engineering to boost up the performance of those advanced MOS devices with extensive industrial applications. As mentioned by Chu et al. in Ref. 6, the viability of novel transistor architectures or channel materials will depend on their ability to provide device enhancement comparable to strained-Si planar MOSFETs. Recently, the fabrication of silicon nanowire transistors with no junctions has been reported.7 In these devices, the channel doping concentration is high with typical values ranging from 1019 to over 5 ⫻ 1019 cm−3. n- and p-channel devices are uniformly doped with donor and acceptor impurities, respectively. The doping type and concentration are the same in the source and drain extensions as in the channel. The absence of doping concentration gradients greatly simpliﬁes fabrication and relaxes thermal budget requirement, especially in ultrashort-channel devices. Those original devices have demonstrated near-ideal subthreshold slope, extremely low leakage current, and less degradation of mobility with gate voltage and temperature than classical transistors. Since the channel of junctionless transistors is heavily doped, one might wonder if straininduced mobility enhancement techniques can be effectively used in these devices. The aim of the present article is to experimentally analyze the impact of mechanical strain on drive current for n- and p-type junctionless Si nanowire MOSFETs. The piezoresistance coefﬁcients 共兲 of doped bulk silicon can be found in the literature.8 The piezoresistance factor in silicon decreases when the doping concentration is in-
creased above 5 ⫻ 1017 cm−3 in n-type silicon and when it is increased above 2 ⫻ 1017 cm−3 in p-type silicon. The reduction of piezoresistance coefﬁcients in n- and p-type silicon is shown in Table I for some typical doping concentrations used in the channel of junctionless transistors. To the reduction of piezoresistance coefﬁcients corresponds a reduction in straininduced mobility enhancement. Indeed, the piezoresistance coefﬁcient is deﬁned as the normalized change in resistivity with stress, = ⌬ / 共 · 兲, where is the applied stress and is the resistivity which is directly related to the carrier mobility by = 1 / 共qnn + q p p兲. The strain-induced mobility enhancement 共L兲 can readily be calculated using the data supplied in Ref. 8 and one ﬁnds L = 35.2 cm2 / dyne= 352⫻ 10−6 MPa−1 for p-type silicon and L = 31.2 cm2 / dyne= 312⫻ 10−6 MPa−1 for n-type silicon at a doping concentration of 2 ⫻ 1019 cm−3. The devices were fabricated on standard 共100兲 Unibond SOI wafers with a 340 nm top silicon layer and a 400 nm buried oxide. The starting SOI ﬁlm was p-type with a resistivity of 10– 20 ⍀ cm. The SOI layer was thinned down to 10–15 nm and patterned to form silicon nanowires using e-beam lithography. Nanowires with different widths were patterned, in order to obtain devices with a width ranging between 20 and 40 nm. A 10 nm gate oxide was grown and ion implantation was used to dope the devices uniformly n+ and p+ with a concentration of 2 ⫻ 1019 cm−3 to realize n-channel and p-channel devices, respectively. A 50 nm thick polysilicon layer was deposited by low-pressure chemical vapor deposition on the gate oxide and doped either p++ for TABLE I. Reduction of piezoresistance coefﬁcient 共in percents兲 in n-type and p-type silicon for some values of doping concentration used in the channel of junctionless transistors.
Electronic mail: [email protected]
Tel.: ⫹32 10 47 23 09, FAX: ⫹32 10 47 87 05. b兲 Electronic mail: [email protected]
Tel.: ⫹353 21 490 48 65, FAX: ⫹353 21 420 57 03. a兲
1 ⫻ 1019 cm−3 2 ⫻ 1019 cm−3 5 ⫻ 1019 cm−3
14% 26% 46%
30% 51% 71%
© 2010 American Institute of Physics
Appl. Phys. Lett. 97, 042114 共2010兲
Raskin et al.
FIG. 1. 共Color online兲 Four-point bending measurement setup and relationship between the induced stress 共兲 and vertical displacement 共y兲 of the bottom movable rods. For all measurements, the spacing “a” was equal to 20 mm.
nMOS devices or n for pMOS devices. The devices studied here have a gate length of 1 m. No source or drain implant was performed on the junctionless MuGFETs. Oxide was deposited and etched to form contact holes, and TiW + aluminum metallization completed the process. The channel of the devices follows the 具110典 crystal direction. Mobility measurements made using the maximum of transconductance method yield mobility values in the range 80– 100 cm2 / V s for both electrons in n-channel devices and holes in p-channel device.9 Unlike inversion-mode and accumulation-mode MuGFETs, junctionless transistors in the on-state operate by bulk conduction 共i.e., not surface channel conduction兲. Thus, their piezoresistance coefﬁcients and mobility enhancement effects must be compared to bulk silicon values.8 The devices were measured using a wafer probe system equipped with a four-point bending setup that allows for bending the wafers in order to generate uniaxial strain in the transistors.4 Bending the center of the wafer upwards creates a tensile stress on the top ﬁber of the wafer, and bending it downwards creates a compressive stress 共Fig. 1兲. The transfer and output characteristics were measured for various devices geometries and applied stress values. The maximum stress is limited to 150 MPa to avoid breaking the wafers. This experimental setup provides a simple way to gain conﬁdence in the effect of strain on transistor performance without modifying the process ﬂow. This is quite important since many process ﬂow parameters are changed when fabricating strained MOSFETs, there is thus uncertainly as to whether
FIG. 3. 共Color online兲 The variation in drain current, ⌬ID / ID, as a function of applied tensile stress in a n-type junctionless MuGFET with a ﬁn width of 30 nm.
strain is the unique responsible for performance enhancement. The stress is applied in 具110典 crystalline direction, i.e., parallel to the current ﬂow in the devices. Compression and traction stresses are, respectively, applied to p- and n-type junctionless MuGFETs. The devices were measured for a gate voltage ranging from 0.4 to 1.1 V 共n-channel, VTH = −0.8 V兲 and –0.6 to –1.8 V 共p-channel, VTH = +0.2 V兲. The variation in drain current, ⌬ID / ID, as a function of the applied stress is plotted for p-共compression兲 and n-共traction兲 type junctionless MuGFETs in Figs. 2 and 3, respectively. The ﬁn width of those devices is 30 nm and the gate voltage overdrive, VGS-VTH, considered for the current extraction is 0.5 V. At least ﬁve devices for each stress level were measured. The characteristic ﬂuctuation between devices is represented by a vertical bar in the graphs for each stress level. This ﬂuctuation is pretty low, especially for p-type junctionless MuGFETs. The origin of this scattering might be of course related to the variability between devices but also to the measurement accuracy in terms of actual applied stress. The bars are more important for low level of applied stress. In fact, the main source of inaccuracy comes from the operator ability to deﬁne the zero point, = 0 MPa. For this particular measurement point, the pressure applied between the two bottom metallic rods and the metallic back side of the Si wafer must be sufﬁcient to assure a good ground contact but cannot induce bending of the wafer. In both cases, we observe a linear increase in the drain current relative change as a function of stress. From the slope of represented straight lines in Figs. 2 and 3, the longitudinal piezoresistance factors, L, are extracted for, respectively, pand n-type junctionless MuGFETs. The results are summarized in Table II and are found to be in excellent agreement with the theoretical values proposed by Kanda.8 TABLE II. Piezoresistance coefﬁcients in n-type and p-type devices. The calculated values are taken from Ref. 8 for a doping concentration of 2 ⫻ 1019 cm−3.
FIG. 2. 共Color online兲 The variation in drain current, ⌬ID / ID, as a function of applied compression stress in a p-type junctionless MuGFET with a ﬁn width of 30 nm.
L measured 共MPa−1兲
L calculated 共MPa−1兲
233⫾ 25⫻ 10−6 333⫾ 10⫻ 10−6
230⫻ 10−6 352⫻ 10−6
Appl. Phys. Lett. 97, 042114 共2010兲
Raskin et al.
agreement with the published piezoresistance coefﬁcients for bulk silicon. A constant mobility enhancement factor is obtained over the whole gate bias range of interest in on-state. The combination of strained SOI and junctionless concept should lead to high-performance nanowire complementary MOS devices.
FIG. 4. 共Color online兲 The variation in drain current, ⌬ID / ID, as a function of gate voltage overdrive, VGS-VTH, in a p-type junctionless MuGFET characterized by ﬁn width of 20, 30, or 40 nm for various applied compressive stresses.
Figure 4 shows the variation in drain current, ⌬ID / ID, as a function of the gate voltage overdrive for p-type MuGFET characterized by ﬁn width of 20, 30, or 40 nm and for applied compressive stress of 50, 100, or 150 MPa. No variations with the ﬁn width demonstrate that there is no lateral geometry conﬁnement on the piezoresistance effect. Contrary to classical planar or nonplanar MOSFETs working in inversion regime, the current relative change, ⌬ID / ID, is nearly independent on gate voltage overdrive for each recorded stress value. This beneﬁcial behavior is directly related to the bulk conduction mode of junctionless MOSFETs. It means strain channel engineering improves carrier mobility over the whole gate bias range in on-state whereas for inversion mode strained-transistors the mobility enhancement degrades with gate voltage overdrive. In conclusion, improvement of current drive using strain in junctionless n- and p-type nanowire MOSFETs is demonstrated. The extracted piezoresistance coefﬁcients are in good
This work is supported by the Science Foundation Ireland under Grant No. 05/IN/I888, Advanced Scalable Silicon-on-Insulator Devices for Beyond-End-of-Roadmap Semiconductors. This work has also been enabled by the Programme for Research in Third-Level Institutions. This work was supported in part by the European Community 共EC兲 Seventh Framework Program through the Networks of Excellence NANOSIL and EUROSOI+ under Contract Nos. 216171 and 216373. 1
S. E. Thompson, M. Armstrong, C. Auth, S. Cea, R. Chau, G. Glass, T. Hoffman, J. Klaus, Z. Ma, B. McIntyre, A. Murthy, B. Obradovic, L. Shifren, S. Sivakumar, S. Tyagi, T. Ghani, K. Mistry, M. Bohr, and Y. El-Mansy, IEEE Trans. Electron Devices 51–4, 191 共2004兲. 2 R. E. Belford, J. Electron. Mater. 30, 807 共2001兲. 3 S. Takagi, T. Mizuno, T. Tezuka, N. Sugiyama, T. Numata, K. Usuda, Y. Moriyama, S. Nakaharai, J. Koga, A. Tanabe, and T. Maeda, Appl. Surf. Sci. 224, 241 共2004兲. 4 F. Rochette, M. Cassé, M. Mouis, A. Haziot, T. Pioger, G. Ghibaudo, and F. Boulanger, Solid-State Electronics 53, 392 共2009兲. 5 N. Serra, F. Conzatti, D. Esseni, M. De Michielis, P. Palestri, L. Selmi, S. Thomas, T. E. Whall, E. H. C. Parker, D. R. Leadley, L. Witters, A. Hikavyy, M. J. Hÿtch, F. Houdellier, E. Snoeck, T. J. Wang, W. C. Lee, G. Vellianitis, M. J. H. van Dal, B. Duriez, G. Doornbos, and R. J. P. Lander, Tech. Dig. - Int. Electron Devices Meet. 2009, 71. 6 M. Chu, Y. Sun, U. Aghoram, and S. E. Thompson, Annu. Rev. Mater. Res. 39, 203 共2009兲. 7 J.-P. Colinge, C. W. Lee, A. Afzalian, N. Dehdashti Akhavan, R. Yan, I. Ferain, P. Razavi, B. O’Neill, A. Blake, M. White, A. M. Kelleher, B. McCarthy, and R. Murphy, Nat. Nanotechnol. 5, 225 共2010兲. 8 Y. Kanda, IEEE Trans. Electron Devices 29, 64 共1982兲. 9 C. W. Lee, A. Borne, I. Ferain, A. Afzalian, R. Yan, N. Dehdashti, and J.-P. Colinge, IEEE Trans. Electron Devices 57, 620 共2010兲.